Australian Asphalt Pavement Association – 2010 1
These notes are based substantially on the text of the Austroads Asphalt Guide. For more detailed
information, users are referred to the Asphalt Guide and other referenced publications.
During the asphalt paving operation, compaction is a two-stage process, as follows:
1. Primary compaction by the paver screed
2. Secondary compaction by rollers.
This section deals with secondary compaction by rollers and supplementary devices for areas
inaccessible to rollers.
Adequate compaction of asphalt is essential to ensure the design performance of the mix and
expected service life is achieved. The compaction should be uniform and achieve a high density.
Mix properties that are directly related to the achievement of adequate density include:
strength, both compressive and shear
resistance to oxidation and ravelling
resistance to rutting
surface texture and appearance
The main factors influencing the successful compaction of asphalt are:
rolling procedures and techniques
temperature of the mix
soundness and stiffness of the underlying base
type and numbers of rollers or other compaction equipment.
The underlying base must be sufficiently sound and rigid to uniformly distribute the stresses from
the compaction equipment without distortion. In the event that the underlying base is inadequate for
the type of mix and compaction equipment being used, the resultant surface may be uneven and
cracked, and the asphalt thickness and density non-uniform.
2 Compaction Equipment
The compaction equipment for asphalt work includes:
non-vibratory (“static”) steel-wheeled rollers
vibratory steel-wheeled rollers (Figure 1)
pneumatic-tyred rollers (Figure 2)
impact compactors such as vibratory plates (Figure 3), hand tampers, etc. (minor works only).
The condition of rollers used for asphalt work can have a significant effect on the finished surface.
To be suitable for asphalt work, the compacting surfaces of the equipment must be true and free
It is important that rollers are properly maintained. With pneumatic-tyred rollers, the tyre pressures
should be even and wheel bearings in good condition to avoid uneven tyre load and resulting
differential compaction of the mix. Adequate ballast should also be used.
2 Australian Asphalt Pavement Association – 2010
Rollers should have good brakes and smooth transmission systems to prevent shoving damage to
the mix when starting, stopping and changing direction. The steering should also be in proper
To prevent pick-up of the mix, rollers should be fitted with watering systems and fibre mats or
scrapers. Care should be taken not to use excessive amounts of water, which may cool the
asphalt. Once the tyres of pneumatic-tyred rollers have heated up, the water may not be required.
Figure 1 Vibratory steel-wheeled roller
Figure 2 Pneumatic-tyred rollers
Australian Asphalt Pavement Association – 2010 3
Figure 3 Vibratory plate
Mechanical tampers, vibratory plates, hand guided rollers and hand tampers are used mainly on
small jobs, or in areas where it is difficult to obtain access for larger rollers, e.g. median nosings.
Light applications of diesel oil on this compaction equipment may also be used to prevent pick-up.
The use of excessive diesel should be avoided, as it will soften the asphalt.
3 Mix Temperatures for Placing
Asphalt must be compacted while it is in a workable state.
The major factors in workability or compactability are:
internal friction, determined by maximum aggregate particle size, particle size distribution and
viscosity of the binder, which affects internal cohesion and the shear resistance.
Generally, mixes with coarse gradings, fully crushed aggregates and larger aggregate sizes are
more stable and require greater compactive effort.
Viscosity of the binder is a function of temperature and binder type. Temperature is by far the most
important factor and a key element in the compactability of the asphalt mix.
The mix should not, however, be so hot as to result in a low viscosity of binder and insufficient
cohesion in the mix to adequately support rollers without excessive displacement.
Temperature of asphalt during placing will depend on the initial spreading temperature and rate of
The rate of cooling is a function of:
road surface temperature
ambient conditions – air temperature, wind, and moisture.
Thicker layers retain the heat longer, resulting in more time for compaction and/or a reduced
number of passes. Retention of heat in thick layers may also lead to a need to delay placing of
subsequent layers until the lower layer has cooled sufficiently to provide a solid working platform.
Asphalt will cool more rapidly at low base temperatures. Wind and rain will further increase the rate
Asphalt mixes containing modified bitumen binders generally require compaction to be completed
at temperatures that are typically 5°C to 10°C higher than mixes with conventional binder, as the
binder stiffens more quickly. Most manufacturers of PMBs provide guidelines for their particular
All these factors are inter-related and influence:
conditions under which asphalt work should proceed
4 Australian Asphalt Pavement Association – 2010
minimum temperature for delivery and spreading of asphalt
time available for compaction and hence choice of rolling equipment and compaction
Table 1 provides a guide to minimum temperatures for spreading dense graded asphalt mixes
based on road surface temperature and layer thickness, using conventional bitumen binders and
conventional compaction techniques.
Table 1 Asphalt spreading temperatures
Minimum mix temperature2 (°°C) Range of mix
Thickness of layer, mm
< 30 30 - 40 41 -100 > 100
5 - 10 See note 4 See note 4 145 135 - 150
10 – 15 150 145 140 130 – 145
15 – 25 150 145 135 125 – 140
> 25 150 145 130 120 – 135
1. Surface temperature should be generally that applicable to the coolest area of the pavements, e.g. shade
areas, if applicable
2. Mix temperatures apply to dense graded mixes with Class 170 and 320 bitumen binder. Use of Class
600, Multigrade, or PMBs may require minimum temperatures 5°C to 10°C higher than those shown.
The need to avoid binder drain-off in open graded mixes may result in temperatures of up to 15°C less
than dense graded mixes.
3. The upper limit of temperature of thick layers is applied to avoid excessive displacement under rolling.
4. Placing asphalt in thin layers under cool conditions may adversely affect the result due to the increased
difficulty in achieving proper compaction, effective joints and good surface finish. Additional attention
should be paid to issues of mix workability, asphalt temperature, compaction techniques and any
influence from additional cooling due to wind or moisture.
Table 2 provides a guide to typical asphalt mix temperatures related to critical binder viscosities for
different stages of compaction (Section 6).
The table is based on the following nominal viscosity levels:
Mixing – a viscosity of around 0.1 Pa.s provides a binder of a suitable consistency for mixing
with aggregates, and also tends to be around the maximum temperature for production and
Binder drainage in OGA – Binder drainage will be influenced by binder content, filler content
and use of fibres (Section 4.13). Without fibres, the risk of drainage is increased if the binder
viscosity is less than about 0.12 Pa.s.
Maximum compaction temperature – The asphalt mix must have sufficient cohesion to support
rolling equipment without excessive displacement. This is typically a binder viscosity of around
Minimum compaction temperature – this is the minimum temperature at which initial rolling by
steel rollers remains effective and typically occurs at around 10 Pa.s, although some PMBs
may continue to be compacted at slightly higher binder viscosities.
Minimum for final rolling – Minimum temperature at which intermediate and final rolling is
effective. This typically occurs at around 100 Pa.s.
Softening point – Typical values are provided for reference and generally represent a viscosity
of around 1200 Pa.s.
Australian Asphalt Pavement Association – 2010 5
Table 2 Typical temperatures for placing and compacting of asphalt
containing various binders
170 45 65 90 140 150 160